KUO, C-Y., DREES, Y., FERNÁNDEZ-DÍAZ, M.T., ZHAO, L., VASYLECHKO,
L., SHEPTYAKOV, D., BELL, Anthony, PI, T.W., LIN, H-J., WU, M-K.,
PELLEGRIN, E., VALVIDARES, S.M., LI, Z.W., ADLER, P., TODOROVA, A.,
KÜCHLER, R., STEPPKE, A., TJENG, L.H., HU, Z. and KOMAREK, A.C.
Available from Sheffield Hallam University Research Archive (SHURA) at:
This document is the author deposited version. You are advised to consult the
publisher's version if you wish to cite from it.
KUO, C-Y., DREES, Y., FERNÁNDEZ-DÍAZ, M.T., ZHAO, L., VASYLECHKO, L.,
SHEPTYAKOV, D., BELL, Anthony, PI, T.W., LIN, H-J., WU, M-K., PELLEGRIN, E.,
VALVIDARES, S.M., LI, Z.W., ADLER, P., TODOROVA, A., KÜCHLER, R.,
STEPPKE, A., TJENG, L.H., HU, Z. and KOMAREK, A.C. (2014). k=0Magnetic
Structure and Absence of Ferroelectricity in SmFeO3. Physical Review Letters, 113
Copyright and re-use policy
Sheffield Hallam University Research Archive
0 Magnetic Structure and Absence of Ferroelectricity in
C.-Y. Kuo,1 Y. Drees,1 M. T. Fernández-Díaz,2 L. Zhao,3 L. Vasylechko,1,4 D. Sheptyakov,5 A. M. T. Bell,6 T. W. Pi,7H.-J. Lin,7 M.-K. Wu,3 E. Pellegrin,8 S. M. Valvidares,8 Z. W. Li,1 P. Adler,1 A. Todorova,1
R. Küchler,1 A. Steppke,1 L. H. Tjeng,1 Z. Hu,1 and A. C. Komarek1,*
Max-Planck-Institute for Chemical Physics of Solids, Nöthnitzer Strasse 40, 01187 Dresden, Germany
2Institut Laue-Langevin, 38042 Grenoble, France 3
Institute of Physics, Academia Sinica, Taipei 11529, Taiwan
4Lviv Polytechnic National University, 12 Bandera Street, 79013 Lviv, Ukraine 5
Laboratory for Neutron Scattering and Imaging, Paul Scherrer Institut, CH-5232 Villigen PSI, Switzerland
6HASYLAB at DESY, Notkestrasse 85, 22607 Hamburg, Germany 7
National Synchrotron Radiation Research Center (NSRRC), 101 Hsin-Ann Road, Hsinchu 30077, Taiwan
8CELLS-ALBA Synchrotron Radiation Facility, Carretera BP 1413, km 3.3, E-08290 Cerdanyola del Vallès, Barcelona, Spain
(Received 18 June 2014; published 20 November 2014)
SmFeO3 has attracted considerable attention very recently due to its reported multiferroic properties above room temperature. We have performed powder and single crystal neutron diffraction as well as complementary polarization dependent soft X-ray absorption spectroscopy measurements on floating-zone grown SmFeO3 single crystals in order to determine its magnetic structure. We found ak¼0 G-type collinear antiferromagnetic structure that is not compatible with inverse Dzyaloshinskii-Moriya interaction driven ferroelectricity. While the structural data reveal a clear sign for magneto-elastic coupling at the Néel-temperature of ∼675K, the dielectric measurements remain silent as far as ferroelectricity is concerned.
DOI:10.1103/PhysRevLett.113.217203 PACS numbers: 75.25.-j, 61.05.fg, 75.85.+t, 77.22.-d
The discovery of magnetism induced ferroelectricity has renewed interest in multiferroic materials due to the enhanced magnetoelectric interaction in these materials that makes them very interesting for technical applications [1,2]. Recently, it has been found that ferroelectricity can arise from some special types of magnetic structures inducing sizeable magnetoelectric effects and the ability to switch the electric polarization by an applied magnetic field (and vice versa). In these recently studied materials, magnetic frustration induces a complex magnetic structure with cycloids or spirals . However, also the ordering temperatures need to be above room temperature in order to make these materials interesting for technical applications. Very recently, the discovery of ferroelectric polarization in SmFeO3has been reported belowTN∼670K. The origin of this ferroelectric polarization is highly debated [3–5]. A further spin-reorientation transition occurs at TSR∼ 480K in this material without having any noticeable effect on the ferroelectric polarization. In the initial publication an inverse Dzyaloshinskii-Moriya interaction based mecha-nism has been reported to be the driving force of the ferroelectric properties of SmFeO3 . The underlying
k¼0 magnetic structure was not directly measured but calculated by ab initio calculations . However, it has been demonstrated that this calculated k¼0 magnetic structure with magnetic ions located at inversion centers cannot be responsible for a spin-orbit-coupling driven ferroelectric polarization bySi×Sj in this material since inversion symmetry will not be broken . Within this
context, an alternative mechanism based on JSi•Sj
exchange-striction has been proposed to be responsible for the ferroelectric polarization in SmFeO3 .
Here, we report the experimentally observed magnetic structure of SmFeO3and reanalyze the ferroelectric proper-ties of SmFeO3. A large reddish SmFeO3single crystal with
TN∼675 K has been grown at a Crystal Systems Corp. 4-mirror optical floating zone furnace. The high sample quality of this insulating reddish orange single crystal has been confirmed by EDX, Laue, and x-ray diffraction techniques as well as by magnetization and Mössbauer spectroscopy measurements; see the Supplemental Materials
. In the inset of Fig.1(a)a polarization microscope image
is shown that indicates—together with our Laue diffraction analysis—that our SmFeO3crystals are single domain single crystals. No impurity phases are visible in highly accurate synchrotron radiation powder x-ray diffraction measure-ments that have been performed at beamline B2 of DORIS-III at DESY. The lattice parameters, unit cell volume and relative expansion of the lattice parameters of SmFeO3 (Pbnm setting with a < b < c) are shown in Figs. 1(a),
1(b). The b-lattice parameter exhibits a small anomalous
kink around TN that is indicative for magnetoelastic cou-pling at the magnetic ordering temperature TN. The other lattice parameters exhibit much less pronounced anomalies atTN that are even only barely visible in the derivatives of the lattice parameters; see Figs.1(c),1(d).
experimental determination of the magnetic structure of SmFeO3. Here, we present two complementary neutron measurements where we were able to overcome these obstacles and measure the magnetic structure of SmFeO3 directly. First, we have performed powder neutron diffrac-tion measurements at comparably low neutron energies (λ¼1.8857Å) with a special sample geometry at the HRPT diffractometer (SINQ). We were able to overcome the highly neutron absorbing properties of Sm by filling the
outer volume of a hollow vanadium cylinder with a special mixture of fine SmFeO3powder that we“diluted”with fine aluminum powder in order to suppress the Sm absorption effects. As can be seen in Fig.2, we obtained qualitatively good powder neutron diffraction patterns at 300, 515, and 720 K that could be easily refined with two additional phases of Al and V which do not interfere at all with the SmFeO3 magnetic signal and barely interfere with structural contri-butions. Therefore, a reliable Rietveld refinement of the magnetic structure of SmFeO3 could be performed.
Since we measured only at temperatures above room temperature, we neglected any Sm ordering. As pointed out in great detail in Ref. , there are four different irreducible representationsΓþ1,Γþ2,Γþ3, andΓþ4 correspond-ing to the followcorrespond-ing four spin configurations for the Fe ordering: AxGyCz, GxAyFz, FxCyGz and CxFyAz which correspond to the magnetic space groupsPbnm,Pb0n0m,
Pbn0m0 and Pb0nm0, respectively . Our neutron mea-surements at 300, 515, and 720 K clearly show that there appearsFxCyGz-type andGxAyFz-type antiferromagnetic ordering in SmFeO3 at 300 and 515 K, respectively. The Rietveld fits of the magnetic intensities are shown in Fig. 2 and the corresponding magnetic moments are listed in Table I in the Supplemental Material. Other spin configurations or incommensurate magnetic structures can be excluded for SmFeO3. We have also performed complementary single crystal neutron diffraction measure-ments. By choosing an optimized small sample geometry and high incident neutron energies we were able to perform single crystal neutron diffraction measurements at the D9 diffractometer (ILL). The temperature dependence of some prominent magnetic intensities are shown in Fig.3(a)
FIG. 2 (color online). Powder neutron diffraction measure-ments of SmFeO3 at (a),(b) 300 K and at (c),(d) 515 K. Blue circles: measured intensities, black line: Rietveld fit, green line:
Iobs−Ical, red line: measured intensities in the paramagnetic
phase at 720 K, gray and magenta bars: nuclear and magnetic peak positions, respectively.
FIG. 1 (color online). Results of our synchrotron radiation powder x-ray diffraction measurements of SmFeO3 obtained at beam line B2 of DORIS-III at DESY (λ¼0.538163Å, space group Pbnm). (a) Relative expansion rðaÞ ¼ ½aðTÞ−
að300KÞ=að300 KÞ. In the inset a polarization microscope image of a single crystalline sample is shown. (b) Unit cell volume and pseudocubic lattice parameters Vc¼V=4, ac¼a=
, cc¼c=2. (c)–(e) The derivative
dac=dT of the pseudocubic lattice parameters (averaged over 4
data points). All dashed lines are guide to the eyes.
visualizing the spin-reorientation transition. The atomic positions derived from this measurement are very close to the atomic positions derived from a complementary single crystal x-ray diffraction measurement that has been per-formed on a Bruker D8 VENTURE x-ray diffractometer as well as with values given in literature, thus, proving the high reliability of our neutron measurements; see Table I in the Supplemental Material . The comparably good refinement statistics and R values of the structure refine-ment of this single crystal neutron measurerefine-ment are shown in Fig.3(b)and Table I in the Supplemental Material . Finally, we were able to determine the magnetic structure of SmFeO3 and observe a collinear k¼0 antiferromagnetic structure; see Figs. 3(c), 3(d). The detection of very tiny canted magnetic moments is beyond the scope of these measurements. As pointed out in Ref.for SmFeO3(with magnetic ions located at inversion centers),k¼0magnetic structures are not compatible with an inverse Dzyaloshinskii-Moriya interaction induced electric polarization.
The antiferromagnetic properties of SmFeO3 were also studied by linear polarization dependent Fe-L edge x-ray absorption spectra (XAS), conducted at 08B beam line of the National Synchrotron Radiation Research Center (NSRRC) in Taiwan. The spectra were recorded with the total electron yield mode using Fe2O3for calibration. X-ray magnetic linear dichroism (XMLD) is the difference in cross section for light polarized perpendicular or parallel to the magnetic moment and is well known to be sensitive to the spin direction of antiferromagnetic systems [11–13]. We have measured the polarization dependent Fe-L2XAS spectra at 440 and 490 K with the Poynting vector of the light being parallel to the a, b, and c axis shown in Figs. 4(a)–4(c). We observe a considerable size of the XMLD signals between the electric fieldE∥bandE∥cin
Fig.4(a), betweenE∥aandE∥cin Fig.4(b), but nearly no
difference betweenE∥aandE∥bin Fig.4(c). The sign of the XMLD signals is reversed when going from 440 to 490 K; see Figs.4(a),4(b). This is similar to the previous study of the Morin transition of hematite revealing a rotation of the spin orientation acrossTSR. To extract the orientations of the antiferromagnetic axes we have simu-lated the experimental spectra using configuration inter-action cluster calculations. The calculated spectra are shown in Figs.4(a)–4(c) and the parameters used in our calculation are listed in Ref. . The corresponding FeO6 cluster considered in our calculations is also shown in the right part of each figure. One can see that the experimental spectra are nicely reproduced by the calcu-lated spectra with spins parallel to c and a axis at 440 and 490 K, respectively, thus, corroborating the collinear magnetic structure obtained in our neutron measurements. Also our Fe-L2;3 x-ray magnetic circular dichroism (XMCD) spectra as well as our Mössbauer spectroscopy measurements are fully consistent with the fact that there is only one Fe3þ species in SmFeO3; see the Supplemental Material.
Finally, we measured the anisotropic dielectric properties of single crystalline thin plates of SmFeO3. The capacitance was measured over a range of frequencies with an excitation
300 400 500 600 700 0
ounts (arb. u.)
0 5000 10000 0 5000 10000 (d) (c) (a) F 2 cal c (arb. u.) F2 obs(arb. u.)
refinement statistics D9 (300 K)
a b c
300 K 515 K
FIG. 3 (color online). (a) Temperature dependence of magnetic intensities measured on our SmFeO3 single crystal at the D9 diffractometer. (b) Refinement statistics of our magnetic and crystal structure refinement of SmFeO3at 300 K. (c),(d) Magnetic structures of SmFeO3below and above TSR respectively:
FIG. 4 (color online). Fe L2;3 XAS spectra of SmFeO3.
(a)–(c) The linear polarization dependent XAS spectra measured above and below TSR with incident beam parallel to a, b,
level of 1 V, while the temperature was swept at a slow warming or cooling rate (1–2K=min). As shown in Figs.5(a),5(b)the temperature-dependent dielectric constant with electric field along thebaxis,εbðTÞshows only a broad hump with strong frequency dependence below ∼600K. The dielectric loss, tanδ, rises strongly as the temperature increases. All samples are insulators at room temperature and become slightly conductive at high temperatures (several kΩ at 800 K). No apparent anomalies could be observed inεbðTÞ aroundTN. If an intrinsic ferroelectric transition occurs at
TN, the corresponding anomalies should be observable in both εb and tanδ, irrespective of testing frequencies. Also εaðTÞ and εcðTÞ exhibit no anomalies at TN. Complementary capacitance-voltage (C-V) measurements were carried out for all our samples at room temperature. Fig. 5(c) shows a typicalC-V curve with the electric field
applied along thebaxis. No hysteresis could be observed for SmFeO3 within the experimental resolution (<10−4).
Hence, we can exclude the existence of ferroelectricity in SmFeO3. We interpret the observations in Ref.  differ-ently and suggest that strain could be induced by magneto-eleastic coupling atTNwhich then would be responsible for an artificial observation of a pyrocurrent in thebdirection at TN. Indeed, our synchrotron radiation powder x-ray diffraction measurements reveal anomalies predominantly of theb-lattice parameter of SmFeO3atTN; see Fig.1(d). The hysteresis loop reported to occur at 300 K in Ref. may then be attributed to leakage currents which is absent in our experiment. Perhaps this is related to the different lossy character of flux-grown  and floating zone grown single crystals.
The absence of ferroelectric properties in SmFeO3 is also consistent with thek¼0 magnetic structure that we observed. This has to be contrasted with the case of other isostructural multiferroic materials, like TbMnO3, where non-collinear chiral magnetic structures have been observed. We note that for aG-type antiferromagnetic rare-earth orthoferrite RFeO3, the electric polarization induced by exchange striction is known to occur only below the rare earth magnetic ordering temperature which is two orders of magnitude lower thanTN. If exchange striction would be an important mechanism in SmFeO3one would expect to see also a pyrocurrent signal when the magnetic structure exhibits distinct changes atTSR which is not experimentally observed. Finally, we would like to remark that magnetoelastic effects are not only present in prototypical multiferroic materials like BiFeO3 [19,20] but (across the doping series Bi1−xLaxFeO3 ) also in non-ferroelectric centrosymmetric materials like LaFeO3 [22,23]. Our findings suggest that magnetoelastic effects may also lead to an artificial observation of pyrocurrents and, hence, magnetoelastic coupling can easily be mis-interpreted as a ferroelectric response.
We thank D. I. Khomskii, M. W. Haverkort, and A. Tsirlin for helpful discussions. We thank H. Borrmann and his team for x-ray diffraction measurements. We thank U. Burkhardt and his team for EDX measurements. This work is partially based on experiments performed at the Swiss spallation neutron source SINQ, Paul Scherrer Institute, Villigen, Switzerland. XMCD experiments were performed at the BL29 Boreas beam line at the ALBA Synchrotron Light Facility with the collaboration of ALBA staff.
 T. Kimura, T. Goto, H. Shintani, K. Ishizaka, T. Arima, and Y. Tokura,Nature (London)426, 55 (2003).
 S.-W. Cheong and M. Mostovoy,Nat. Mater.6, 13 (2007).  J.-H. Lee, Y. K. Jeong, J. H. Park, M.-A. Oak, H. M. Jang, J. Y. Son, and J. F. Scott,Phys. Rev. Lett.107, 117201 (2011). FIG. 5 (color online). Dielectric characterization of SmFeO3
with the electric field along the b axis at different testing frequencies. (a) The temperature-dependent dielectric constant εb. (b) The tangent loss tanδ. (c) TheC-V curve of SmFeO3at
room temperature with the corresponding loss data in the inset.
 R. D. Johnson, N. Terada, and P. G. Radaelli, Phys. Rev. Lett.108, 219701 (2012).
 J.-H. Lee, Y. K. Jeong, J. H. Park, M.-A. Oak, H. M. Jang, J. Y. Son, and J. F. Scott, Phys. Rev. Lett. 108, 219702 (2012).
 See Supplemental Material at http://link.aps.org/ supplemental/10.1103/PhysRevLett.113.217203, which in-cludes Refs. [3,7,10], for magnetization, Mössbauer and XMCD measurements as well as data of crystal and magnetic structure refinements.
 M. Eibschutz, S. Shtrikman, and D. Treves,Phys. Rev.156, 562 (1967).
 Y. K. Jeong, J.-H. Lee, S.-J. Ahn, and H. M. Jang, Solid State Commun.152, 1112 (2012).
 E. F. Bertaut,Acta Crystallogr. Sect. A24, 217 (1968).  E. N. Maslen, V. A. Streltsov, and N. Ishizawa, Acta
Crystallogr. Sect. B52, 406 (1996).
 P. Kuiper, B. G. Searle, P. Rudolf, L. H. Tjeng, and C. T. Chen,Phys. Rev. Lett.70, 1549 (1993).
 J. X. Zhang et al.,Phys. Rev. Lett.107, 147602 (2011).  J. C. Yanget al.,Phys. Rev. Lett.109, 247606 (2012).
 A. Tanaka and T. Jo,J. Phys. Soc. Jpn. 63, 2788 (1994).  FeO6 cluster parameters [eV]: Udd¼5.0, Upd¼6.0,
Δ¼3.0,10Dq¼1.2,Δeg¼0.04,Δt2g¼0.02,Du¼−0.015, EgMix¼0.02, pdσ¼−1.4, and pdπ¼0.64, Slater
integrals 75% of Hartree-Fock values.
 J. F. Scott,J. Phys. Condens. Matter20, 021001 (2008).  R. Kajimoto, H. Yoshizawa, H. Shintani, T. Kimura, and
Y. Tokura,Phys. Rev. B70, 012401 (2004).
 Y. Tokunaga, N. Furukawa, H. Sakai, Y. Taguchi, T.-h. Arima, and Y. Tokura,Nat. Mater. 8, 558 (2009).  S. Leeet al.,Phys. Rev. B88, 060103 (2013).  J. Parket al.,J. Phys. Soc. Jpn.80, 114714 (2011).  C. M. Kavanagh, R. J. Goff, A. Daoud-Aladine, P.
Lightfoot, and F. D. Morrison, Chem. Mater. 24, 4563 (2012).
 G. L. Beausoleil, P. Price, D. Thomsen, A. Punnoose, R. Ubic, S. Misture, and D. P. Butt,J. Am. Ceram. Soc.97, 228 (2014).